Origin of the blueshift of photoluminescence in a type-II heterostructure
© Jo et al.; licensee Springer. 2012
Received: 4 October 2012
Accepted: 14 November 2012
Published: 27 November 2012
Blueshifts of luminescence observed in type-II heterostructures are quantitatively examined in terms of a self-consistent approach including excitonic effects. This analysis shows that the main contribution to the blueshift originates from the well region rather than the variation of triangular potentials formed in the barrier region. The power law for the blueshift, ΔE PL ∝ P laser m , from m = 1/2 for lower excitation Plaser to m = 1/4 for higher excitation, is obtained from the calculated results combined with a rate equation analysis, which also covers the previously believed m = 1/3 power law within a limited excitation range. The present power law is consistent with the blueshift observed in a GaAsSb/GaAs quantum well.
KeywordsQuantum well type-II Blueshift Excitons GaSb GaAs Photoluminescence 71.35.-y: Excitons 78.55.Cr: Photoluminescence of III-V semiconductor 81.15.Hi: Molecular beam epitaxy
Interest has recently been increasing in type-II heterostructures in which electrons and holes are separated in adjacent different materials, thereby forming spatially indirect excitons [1–9]. The wavefunction of the indirect exciton is significantly extended in space compared with that of a direct exciton in a type-I system where both electrons and holes are confined in the same layer, which allows large controllability of the wavefunction distribution. In addition, the long radiative lifetime originating from spatially indirect recombination is attractive for applications such as optical memories [10, 11].
The separation of charge carriers in a type-II system also induces electrostatic potential (Hartree potential), which causes band bending and a resultant significant change in the exciton wavefunction distribution. Experimentally, this band-bending effect has been observed in power-dependent photoluminescence (PL) measurements, in the blueshift of PL peaks with increasing excitation power [1, 2, 5, 6, 12]. The mechanism of this effect has been discussed in terms of a triangular potential model in which photogenerated electrons and holes form a dipole layer, creating a triangular-like potential at the interface . With increasing excitation power, the potential becomes steeper and the quantization energy increases, giving rise to a blueshift of the recombination energy. Following this model, the blueshift is proportional to the cube root of the excitation power, which has been generally accepted for the characterization and distinction of type-II heterostructures.
However, detailed examinations of the observed power dependency sometimes show deviations from the cube root of power law. This is especially noticeable when the excitation power dependence is examined over a wide range. Here, we reexamine the characteristic blueshift in a type-II system using a GaAsSb/GaAs quantum well (QW). We observe that the blueshift does not obey a single-exponent power law, but instead tends to saturate with increasing excitation power. This is analyzed on the basis of a self-consistent band calculation. The dominant contribution to the blueshift originates from the variation of the QW energy level rather than the variation of the triangular potentials formed in the barrier layers, which modifies the cube-root power law.
The sample containing a 6-nm GaAsSb QW was grown on a GaAs(001) substrate by MOMBE. The Sb composition of GaAsSb was set at 8%, which was confirmed by XRD. At this Sb concentration, the band lineup between GaAs and GaAsSb becomes a type-II alignment with holes confined in the GaAsSb well [13, 14]. The excitation power dependence of the PL was measured at 23 K using the 633 nm line of a He-Ne laser with an intensity range of 1 to 100 W cm-2. The incident beam was chopped using an optical chopper to avoid heating.
Results and discussion
Material parameters used for the calculation of a GaAsSb/GaAs QW
To see how the transition energy shifts with the excitation, we calculated the energy shifts of the electron and heavy hole as a function of the sheet charge density Figure 2b. The energy shift of the optical transition, ΔEPL, is given by the difference between the two energy shifts: ΔEPL = ΔEe - ΔEhh. As the sheet charge density increases, both the electron and heavy-hole energy levels monotonically decrease due to the increasing Hartree potential. Furthermore, the heavy-hole energy shift is always larger than the electron energy shift. As a result, the transition energy shift ΔEPL shows a blueshift with increasing excitation. Indeed, this trend is generally true for a type-II structure; the confined carrier (here the hole) is more susceptible to the Hartree potential. This response is partly because the potential well for the electrons is formed at the skirt of the Hartree potential, while holes are affected by the peak height of the Hartree potential. In addition, an increase in the steepness of the triangular well for the electrons raises the quantization energy, compensating for the energy decrease due to the increased well depth.
Again, the sheet charge density ns is a parameter.
with the power factor m’ depending on the excitation power. We show again the experimental PL peak shift in the inset of Figure 3b, along with the new power law. Transition from the low excitation regime (m’ = 1/2) to the high excitation regime (m’ = 1/4) is obvious. Between the two extremes, we can see the conventionally applied m’ = 1/3 power law regime.
We have analyzed the blueshift of the PL peak in a type-II QW. A one-band calculation shows that the blueshift is mainly caused by the energy shift of the confined carrier in the well. More quantitative analysis based on a self-consistent calculation including excitonic effects illustrated the transition from a linear to a sublinear increase in the blueshift with increasing sheet charge density. Combining the calculated result with the carrier rate equation, the blueshift was found to be proportional to the m-th root of the excitation power density, in which m = 1/2 ~ 1/4 and is dependent on the excitation power. The more comprehensive theory presented here predicts the 1/3-power law in the literature over a limited range of carrier density only. The above power law is consistent with the experimental results obtained from a type-II GaAsSb/GaAs QW.
Metal-organic molecular beam epitaxy
This work was supported in part by Hokkaido University and Hokkaido Innovation through Nano Technology Support (HINTS).
- Ledentsov NN, Böhrer J, Heinrichsdorff F, Grundmann M, Bimberg D, Ivanov SV, Meltser BY, Shaposhnikov SV, Yassievich IN, Faleev NN, Kop'ev PS, Alferov ZI: Radiative states in type-II GaSb/GaAs quantum wells. Phys. Rev. B 1995, 52: 14058. 10.1103/PhysRevB.52.14058View Article
- Hatami F, Grundmann M, Ledentsov NN, Heinrichsdorff F, Heitz R, Böhrer J, Bimberg D, Ruvimov SS, Werner P, Ustinov VM, Kop'ev PS, Alferov ZI: Carrier dynamics in type-II GaSb/GaAs quantum dots. Phys. Rev. B 1998, 57: 4635. 10.1103/PhysRevB.57.4635View Article
- Ribeiro E, Govorov AO, Carvalho W, Medeiros-Ribeiro G: Aharanovo-Bohm signature for neutral polarized excitons in type-II quantum dot ensembles. Phys. Rev. Lett. 2004, 92: 126402.View Article
- Madureira JR, de Godoy MPF, Brasil MJSP, Iikawa F: Spatially indirect excitons in type-II quantum dots. Appl. Phys. Lett. 2007, 90: 212105. 10.1063/1.2741601View Article
- Alonso-Álvarez D, Alén B, García JM, Ripalda JM: Optical investigation of type II GaSb/GaAs self-assembled quantum dots. Appl. Phys. Lett. 2007, 91: 263103. 10.1063/1.2827582View Article
- Kawazu T, Mano T, Noda T, Sakaki H: Optical properties of GaSb/GaAs type-II quantum dots grown by droplet epitaxy. Appl. Phys. Lett. 2009, 94: 081911. 10.1063/1.3090033View Article
- Tatebayashi J, Khoshakhlagh A, Huang SH, Dawson LR, Balakrishnan G, Huffaker DL: Formation and optical characteristics of strain-relieved and densely stacked GaSb/GaAs quantum dots. Appl. Phys. Lett. 2006, 89: 203116. 10.1063/1.2390654View Article
- Dheeraj DL, Patriarche G, Zhou H, Hoang TB, Moses AF, Grønsberg S, Helvoort AT, Fimland BO, Weman H: Growth and characterization of wurtzite GaAs nanowires with defect-free zinc blende GaasSb inserts. Nano Lett. 2008, 8: 4459. 10.1021/nl802406dView Article
- Akopian N, Patriarche G, Liu L, Harmand JC, Zwiller V: Crystal phase quantum dots. Nano Lett. 2010, 10: 1198. 10.1021/nl903534nView Article
- Muto S: On a possiblity of wavelength-domain-multiplication memory using quantum boxes. Jpn. J. Appl. Phys. 1995, 34: L210. 10.1143/JJAP.34.L210View Article
- Geller M, Kapteyn C, Muller-Kirsch L, Heitz R, Bimberg D: Hole storage in GaSb/GaAs quantum dots for memory devices. Phys. Stat. Sol. (b) 2003, 238: 258. 10.1002/pssb.200303023View Article
- Suzuki K, Hogg RA, Arakawa Y: Structural and optical properties of type II GaSb/GaAs self-assembled quantum dots grown by molecular beam epitaxy. J. Appl. Phys. 1999, 85: 8349. 10.1063/1.370622View Article
- Ichii A, Tsou Y, Garmire E: An empirical rule for band offsets between III-V alloy compounds. J. Appl. Phys. 1993, 74: 2112. 10.1063/1.354734View Article
- Noh MS, Ryou JH, Dupuis RD, Chang YL, Weissman RH: Band lineup of pseudomorphic GaAs1-xSbx quantum-well structures with GaAs, GaAsP, and InGaP barriers grown by metal organic chemical vapor deposition. J. Appl. Phys. 2006, 100: 093703. 10.1063/1.2363237View Article
- Yu PY, Cardona M: Fundamentals of Semiconductors. 3rd edition. Berlin: Springer; 2005.
- Vurgaftman I, Meyer JR, Ram-Mohan LR: Band parameters for III-V compound semiconductors and their alloys. J Appl Phys 2001, 89: 5815. 10.1063/1.1368156View Article
- Penn C, Schaffler F, Bauer G, Glutsch S: Application of numerical exciton-wave-function calculations to the question of band alignment in Si/SiGe quantum wells. Phys Rev B 1999, 59: 13314. 10.1103/PhysRevB.59.13314View Article
- Fukatsu S, Usami N, Shiraki Y: Luminescence from Si1-xGex/Si quantum wells grown by Si molecular-beam epitaxy. J Vac Sci Technol B 1993, 11: 895. 10.1116/1.586732View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.